Investigation on a Bio-Composite Material as Acoustic Absorber and Thermal Insulation

: In order to limit the anthropic emissions of CO 2 , research is currently investigating new materials for the building sector. The main purpose is the reduction in the embodied energy consumption, especially in the residential sector, and consequently the limitation of the direct and indirect utilization of fossil fuels, for the indoor heating, cooling, and ventilation services. Indeed, the residential sector is a ﬀ ected by a high energy demand, thus the choice of improved materials is fundamental to improve the sustainability. All phases: construction, building life, and dismantling are impacting in terms of resource and energy consumption, both associated with the emissions of pollutants in the atmosphere. The aim of this experimental research is to study the thermal insulation and the acoustic absorption of a material composed by natural lime, water, and shives from sativa hemp, a variety of hemp usable for industrial applications. In order to assess the main characteristics of this material, some specimens have been made according to required shapes and sizes to test them in speciﬁc machines. The results obtained from the tests are compared with the values of similar lime-based materials already available on the market. The comparison shows how, in certain aspects, the lime and hemp shives materials represent a concrete alternative to conventional materials. This completely natural material would like to achieve thermal and acoustic comfort in indoor environments.


Introduction
The adoption of energy saving approaches in the construction sector is called "green building" [1]. In fact, this term is associated with the philosophy, techniques, science, and know-how related to the saving of energy and resources used from "cradle to grave" of a building [2]. The concept was introduced in Europe by the "Directive on the energy performance of buildings" (2010/31/EU) and implemented in subsequent years by all European countries [3]. In Italy, it was converted into law n. 90/2013 [4]. In order to develop this construction technique, it was decided to create a database of case studies. In this way, useful guidelines are created to design and build ever more efficient buildings [5].
Embodied energy reduction allows to preserve the environment by reducing climate-changing emissions substances such as CO 2 [6]. Among the techniques used for this purpose there are: using waste materials from other sectors, recycled materials [7], natural materials [8], and renewable energy [9]. The use of plant-based materials is considered a technique with many future implications in the environmental acoustics sector. These products have cost, weight, and sound absorption characteristics comparable with traditional materials [10].
In addition to the engineering characteristics, innovative materials must be able to make the environment comply with the specifications required by the standards. In Italy, the decree 5 December

Shives: Role in Construction
The benefits obtainable from hemp use are variegated [24]. As an example, its presence guarantees humidity control, due to its hygroscopicity, which allows it to accumulate and release humidity and consequently guarantee good hygrometric conditions in the environment. As an example, glass wool and classic materials do not have this property [25].
In the treatment of the thermal conductivity coefficient, it is necessary to examine the thermal bridges generated in the various areas of the building. This aspect has been studied on various composite materials obtained with a hemp base. Thermal bridges, such as external edges and windows in the wall, are very common and present in every building structure. In both cases, it has been obtained that, with the appropriate construction strategies, such as the accurate stratigraphy of the wall and the presence of wooden elements, thermal bridges can be managed, limiting the heat dispersion [26].
Therefore, the adoption of new materials, such as the hemp-lime composite, requires the realization of specific tests, in order to verify the correct thermal insulation and sound absorption [27]. The possibility of making bricks has been also studied [28,29]. They guarantee greater massiveness than a panel of less thickness. This technique has shown that the load-bearing structure itself guarantees acoustic comfort without further intervention on the wall stratigraphy [30].
From the thermal point of view, there are many studies that affirm the good response of composed material of lime and hemp shives [24,31]. As the material density decreases, the thermal conductivity coefficient decreases as well and, therefore, the wall thermal performance improves. At the same time, there is a limit due to the mechanical strength of the compound. Therefore, an appropriate compromise must be found between mechanical resistance and thermal insulation [32].

Materials and Methods
The compound here considered was made with natural products. The matrix is a white Natural Hydraulic Lime NHL 3.5 according to the UNI EN 459-1 classification [33]. This lime does not contain clinker or cement. Water is used as binder. This type of lime has a low environmental impact since it has a long-life cycle and can be recycled to create new mortars [34].
The filler is shives, obtained by the woody part of the hemp plant without psychotropic effects. The European Industrial Hemp Association (EIHA) reports growing values regarding its cultivation in European territory. This growth is linked to the diffusion of its use in industrial fields, such as textiles, food and construction [35]. In Italy, the cultivation and processing of hemp is regulated by law n. 242 of 2 December 2016 [36].
The experimental protocol focused on the creation of specimens necessary to establish the mechanical, thermal, and acoustic characteristics of the material being tested. The study was divided into three phases:

1.
Preliminary analysis and material preparation 2.
Experimental tests

Preliminary Analysis and Material Preparation
In this phase, all the templates necessary for the specimen's realization were found. Below are the templates (Figure 1) to make thermal tests, mechanical tests, and acoustic tests.
In this phase, the devices necessary for testing were prepared: • Electronic scale; • Tray to calculate apparent density; • Shredder RETSCH SM 100 with 2 mm screen; • Dough utensils. Therefore, the shives were shredded from 6 mm to 2 mm, so it was evenly distributed in specimens, especially in the smaller ones. Finally, the volume of all templates was calculated. In this way, in the screening phase, it was possible to calculate the matrix/filler ratio.

Screening and Specimen's Preparation
In this phase, the characteristics of the specimens were assessed. It was decided to create three different types of material by changing the volume percentage of shives in the compound, namely 5%, 10%, 20%. In all three cases, the mass of water was equal to half of the mass of lime. These concentrations were chosen by considering the most common mixes available in the literature and other previous studies realized at the Department of Engineering of Palermo University [24,28,32,37].
Once the screening phase was over, the specimens were made in the laboratory "for indoor environments and sustainable technologies" of the Engineering Department. The doughs were made to fill the templates to be used. The specimens were classified with the notation "XX-Φ-%-S", assuming that: • XX: indicates the test type to which the sample will be subjected; PA (acoustic test, Prova Acustica in Italian), PT (thermal test, Prova Termica), PM (mechanical test, Prova Meccanica).
• Φ: specimen's diameter (millimetres). This parameter is omitted in the specimens for mechanical tests because they are parallelepiped. • %: hemp shives percentage. • S: specimen's thickness (centimetres). This parameter is omitted in the specimens for mechanical tests since the thickness variation is not necessary for the study.
Thence, when there is only one number after the type of test (PM, PA, PT), only the percentage of hemp shives was indicated, since diameter and thickness do not affect the tests.
Knowing the lime and shives' density and specimen's volume, it was possible to calculate the mass of total dough necessary to create all the specimens for each single percentage. These mass values for each percentage are reported in Table 1. According to the Italian legislation (DM 17 January 2018) [38], the compound must mature for 28 days. The specimens were disarmed 4 days after the realization (see Figure 2), weighed and left to rest until the twenty-eighth day. On the last day, they were weighed again to evaluate the weight percentage loss due to the water evaporation (see data reported in Tables 2-4). The environment thermo-hygrometric conditions during weighing were: Relative humidity: 50-60% • To make the table easier to be read, it is necessary to consider that: • In order to have more truthful values after the experimental tests, it was decided to create more specimens of the same type and mediate the results.

•
The mechanical test specimens are parallelepipeds, 16 cm long, 4 cm high and 4 cm wide. Thence, in their nomenclature both geometric parameters are omitted.
All specimens are subject to weight loss, depending on the shape of the specimens and the hemp percentage. In fact, the weight reduction is between 17 and 27%, except the specimens for high frequency acoustic tests (Φ = 28 mm), which were affected by a limited weight reduction between 6 and 8%. In these smaller specimens, there is less hemp in absolute value and therefore a smaller weight variation compared to larger specimens in which there is much more hemp. The weight loss is only due to the evaporation of the water contained in the specimens; in fact, the thickness of the specimens has not significantly changed. Tables 2-4 report data on weight variation for thermal, mechanical, and acoustic specimens, respectively, indicating the average value and the standard deviation.

Experimental Tests
In this section, the results from the acoustic, thermal, and mechanical tests are reported, considering the three different mixes of hemp and lime.

Acoustic Tests
The tests were carried out in the acoustic laboratory located in the Engineering Department. Following the UNI EN ISO 10534-2 standard [39], the acoustic absorption of specimens was tested using Kundt tubes. The device is made up of two cylinders, having different diameters (100 and 28 mm). The largest one measures the sound absorption coefficient (α) in the frequency range from 100 to 1600 Hz. The smallest one measures in the range from 500 to 10,000 Hz. The main specifics of the Kundt's tube are reported in Table 5 [40]. The test is based on white noise emission that hits the specimen perpendicularly. The specimen attenuates the incident wave, turning it into heat. Thus, the device measures its sound absorption capacity. Although a different test should be performed (for example according to UNI EN ISO 717-2 or ISO 140-12) to evaluate the transmission coefficient, if the material presents a high absorption coefficient, the transmission coefficient is consequently limited, also allowing good performance for the acoustic insulation of impact sounds [41].
The "dBAlphaTest" software, connected to the tube, returns the sound absorption coefficient trend. Among the obtained results, it can be noted that, as the shives percentage increases, α improves following a non-linear trend.
During the experimentation, all specimens, both 3 cm and 4 cm, were tested in the Kundt's tube. To compare the material acoustic response to the variation of the fibre percentage, a graph is given for each type (see Figure 3A-F).   The 20% specimens have the best absorption coefficient compared to the others. This result is due to the greater presence of hemp shives, which favours the transformation of the sound wave into thermal energy. For domestic use, the trend of the material at 20% hemp shives and 3 cm thickness is preferred ( Figure 3E). This because it reaches a peak of 65% around 1000 Hz, which is comparable to the speech range, i.e. the dominant frequency in domestic environments.
The FOX 50 device was used to derive the material thermal conductivity coefficient. The main specifics are reported in Table 6 [46]. A temperature difference is set between the device plates, in this case 15 • C. This ∆T generates a thermal flow Q that passes through the specimen; therefore, it is possible to measure its thermal insulation capacity λ, according to Equation (1).
where s is the thickness of the specimen and A the surface orthogonal to the thermal flow. The tests were repeated three times for each specimen to obtain averaged values over multiple trials. As expected, if the shives percentage increases, the apparent density decreases and the thermal insulation capacity improves, as reported in Table 7.

Mechanical Tests
The mechanical tests have the aim of studying the compression and bending material resistance. These characteristics worsen as the shives content grows, thence a right compromise must be found. This phase was performed in the "materials and structures" laboratory of the Engineering Department in Palermo University. The standard UNI EN 1015-11 was followed for these tests [47]. The bending test was performed by using the "Zwick/Roell Z005" machine, which breaks the specimen through a concentrated load in the middle, setting the load cell at 5 kN. The specifics of Zwick/Roell Z005 machine are reported in Table 8 [48]. During the mechanical test, "testXper II" software drew the graph showing the trend of the lowering as a function of the load. These values were converted to bending strength, f m . (Equation (2)), and deformation, D % . (Equation (3)): where: • F is the maximum load applied to the specimen, in Newton. • l is the distance between the support rollers, in millimetres. • b is the width of specimen, in millimetres. • d is the thickness of the specimen, in millimetres.
where: b base, f lowering, l distance between supports. The bending strength trends for specimens at 5% of hemp shives (Figure 4), 10% of hemp shives ( Figure 5) and 20% of hemp shives ( Figure 6) are shown below.   The results obtained show that the greatest resistance was recorded in the case of the 5% shives material ( Figure 4).
Subsequently, the compression test was carried out using the two parts obtained from the bending test. Following the same procedure, with "TestPilotETM" software, the values of the load impressed in relation to the lowering are obtained. In the same way of the previous test, the parameters are converted into compression strength, f c , and deformation, D % . In detail, the compression strength is given by Equation (4): where F max is maximum force measured during the test and A the surface calculated as the product of the specimen thickness and the machine support. The compression stresses trends for specimens at 5% (Figure 7), 10% ( Figure 8) and 20% (Figure 9) are shown below.
In particular, the graph with the trend of the specimens at 5% shows the values of compressive strength higher than the other two percentages. Here the tested specimens are six and not eight because two accidentally broke after the bending tests.
To get an overview, all the mechanical results have been brought together in a single diagram, for bending and compression, where the average values by percentage are shown ( Figure 10).

Conclusions
An experimentation on this type of topic makes it possible to deal with very current issues such as green building and environmental sustainability. Bio-lime and shives lend themselves well to supporting this topic, being of natural origin and recyclable. Analysing the mixture from an ecological point of view, it turns out that the union of these two natural materials gives benefits: to the environment, because the hemp plant during its life transforms CO 2 into oxygen, thus removing it from the air. The union of lime and hemp gives benefits to the indoor environment because it returns it to healthiness. In fact, lime is often referred to as a "hygrometric lung" of a home, because its high vapor permeability facilitates the transfer of humidity and prevents the development of condensation inside the environment. Thus, mould does not develop, which can be harmful to the occupant's health [49]. Its union with the shives gives birth to a material that can be used in a delicate sector such as that of restoration of heritage buildings.
This aspect combines the need to modernize an ancient structure with the need to make it energetically efficient. In fact, the values of thermal conductivity coefficient between 0.05 and 0.1 W/m are acceptable to achieve good energy savings compared to a non-thermally insulated structure.
We have chosen to compare the values obtained from the experimental study with those of some lime-based plasters that are currently on the market ( Table 6). The comparison considers materials that can be used to create the surface layer of the walls, where otherwise the insulating material would be applied in existing buildings.
The values reported in Table 9 reveal that the mixture in shives lime gives comparable thermomechanical characteristics, and in some cases even better than the products already on the market. The study carried out has shown that the increase in percentage of hemp shives in the mixture allows it to have a material with good performances. As expected, before the thermal test, as the percentage of filler increases, the thermal conductivity decreases more. This improves the insulating effect. This claim is supported by the fact that λ values of 0.01 W/mK are found in the literature. As regards the sound absorption values, it has been shown that they increase as the percentage of hemp shives increases. The material, subject of the evaluation, compared to commercial mortars is often superior, like Table 9 shown.
The results here reported encourage the development of this kind of material, due to its good thermal, mechanical and acoustic properties. There is room for further improvements of all characteristics, considering for example the sizes of hemp shives and their ratio in the mix. Future works will consider the effects on the thermal and acoustic properties due to different levels of environmental humidity, as well as the evaluation of the fire resistance performance, which is an important aspect, especially for heritage buildings.  Funding: This research received no external funding.

Conflicts of Interest:
The authors declare no conflict of interest.